ORIGINAL RESEARCH ARTICLEpublished: 04 July 2014
Decolorization of hair dye by lignocellulosic wastematerials from contaminated watersHabib Zahir1, Michelle Naidoo1, Rada-Mayya Kostadinova1, Karla A. Ortiz2, Rosario Sun-Kou3 andAbel E. Navarro1*1 Science Department, Borough of Manhattan Community College, The City University of New York, New York, NY, USA2 Department of Chemistry, College of Arts and Science, New York University, New York, NY, USA3 Seccin Qumica, Departamento de Ciencias, Pontificia Universidad Catlica del Per, Lima, Per
Edited by:Aziz Ullah, Kohat University ofScience and Technology, Pakistan
Reviewed by:Urs Jans, City College of the CityUniversity of New York, USAFrancesco Di Natale, Universit diNapoli Federico II, Italy
*Correspondence:Abel E. Navarro, ScienceDepartment, Borough of ManhattanCommunity College, 199 ChambersStreet, New York, NY 10007, USAe-mail: email@example.com
Basic yellow 57 (BY57) was chosen as a model hair dye due to its prevalence in cosmeticswastewaters. This study proposes the use of lignocellulosic materials like spent tea leavesof peppermint (PM), chai tea (CT), and chamomile (CM) as raw adsorbents for the removalof BY57 from contaminated solutions. Batch adsorption experiments were carried out atroom temperature to achieve the maximum adsorption capacity. Results indicate that thehighest removal is achieved at pH 68, with a minimum adsorbent mass of 75 mg andin the absence of salinity, crowding agents and heavy metals. Adsorption equilibria weremodeled according to the Langmuir and Freundlich isotherm theories and reported thefollowing trend: PM > CT > CM, reaching qmax values of 105, 80, and 38 mg of dye pergram of adsorbent, respectively. Desorption experiments showed that diluted solutionof HCl is able to desorb up to 80% of the dye and recover the adsorbent to be usedin consecutive cycles. Finally, the adsorbents were characterized by Scanning electronmicroscopy (SEM), indicating that the adsorbents have a porous and heterogeneoussurface, showing pockets and protrusions that are potential adsorption sites for the dye.
Keywords: adsorption, basic yellow 57, tea leaves, pH, desorption, isotherm
INTRODUCTIONDifferent substances are currently used as coloring agents. Theycan be divided into two big groups, dyes, and pigments thatare soluble and insoluble in water, respectively. Dyes can bedefined as substances that confer color without being affectedby factors like light, water, and surfactants. Their structure isformed by more than one type of functional groups, mainly aro-matic rings that can be nitro-, amino-, and hydroxyl-substituted(Singh-Rai et al., 2005). Since 1856, more than 10,000 typesof colorants have been produced. Today, more than 7 105Tons of dyes are produced per year, and more than 10% is lostduring the industrial dyeing process (Zollinger, 1991; Easton,1995).
Dyes contain chromophores of high molar mass thataccumulate in lakes and bays; and promote a decrease in the pho-tosynthetic activity. This also causes a decrease in the availableoxygen content, and favors eutrophication processes due to theincrease of organic matter (Robinson et al., 2001).
There are several types of chemical and physical processes forthe removal of dyes, such as ozonation, oxidative degradation,photochemical processes, bleaching, electrochemical degrada-tion, adsorption, treatment with activated carbon, microfiltra-tion, ionic exchange, irradiation, amongst others (Volesky, 2004;Liu and Wang, 2009; Navarro et al., 2013). Although these tech-niques have been conventionally used for the removal of dyes andother pollutants; they still show important disadvantages suchas high operative costs and generation of byproducts that need
further treatment (Robinson et al., 2001; Kotrba et al., 2011; Kimet al., 2013).
Biological treatment by activated sludge has been successfullyused for the treatment of dye-containing wastewaters and iswidely used in water purification plants. Bioaccumulation hasalso been applied to the decontamination of pollutants, by usingmicroorganisms such as bacteria, algae, yeast, and fungi (Guoet al., 2008; Gonzalez and Fuentes, 2009; Kotrba et al., 2011). Themost important advantage of microorganisms is their selectivityin the uptake of pollutants. However, they also show drawbackslike adequate temperature, enough nutrients, and constant agi-tation for their operation (Liu and Wang, 2009; Kotrba et al.,2011). Conversely, biosorption utilizes dead biomass like spenttea leaves, dead algae, crustacean shells, eggshells, and other bio-logical residues to eliminate pollutants. The removal is throughadsorption that is mainly driven by intermolecular interactionslike electrostatic, hydrogen bonding, dipole dipole, and disper-sion forces (Liu and Wang, 2009; Iparraguirre et al., 2010; Kimet al., 2013; Navarro et al., 2013). Spectroscopic studies haveshown that these biosorbents have active adsorption sites suchas carboxyl, hydroxyl, and amino groups on their surfaces. Ithas been demonstrated that all these groups have a great affin-ity toward pollutants like heavy metals (Cuizano et al., 2009; Diazet al., 2013), phenols (Navarro et al., 2008a,b), and dyes (Naidooet al., 2013; Navarro et al., 2013).
Basic yellow 57 (BY57) hair dye is commonly used in cosmeticsin the formulation of hair coloring pastes. As shown in Figure 1, it
www.frontiersin.org July 2014 | Volume 2 | Article 28 | 1
Zahir et al. Inexpensive decolorization by lignocellulosic materials
FIGURE 1 | Chemical structure of the cationic dye Basic Yellow 57(BY57).
is a cationic dye with polar groups like amide, quaternary amine,azo, and heterocyclic rings. BY57 is water soluble at any pH andin the presence of other organic and inorganic solutes.
The purpose of this study is the use of lignocellulosic wastematerials like spent peppermint (PM), chai tea (CT), andchamomile (CM) teas on the removal of BY57 from contam-inated solutions. These spent teas are massively discarded bytea-based industries and become a waste disposal concern. Wepropose that this industrial waste can be recycled and used as eco-friendly adsorbents. Our long term goal envisions the preparationof recyclable filters in continuous-flow industrial processes for theremoval of BY57 and other dyes and organic pollutants.
MATERIALS AND METHODSDYE SOLUTIONSStock solution of BY57 was prepared by dissolving the dye indeionized water and brought to a concentration of 1000 mg/L.BY57 dye was donated by Vanshi Chemicals Pvt Ltd. (India).Solutions of varying concentrations were prepared by dilution ofthe stock with deionized water. The initial pH of the solutionswere measured with a pH-meter (Fisher Scientific, AccumetAB15) and adjusted to the required pH value by adding aliquotsof concentrated HCl and NaOH solutions prior contact with theadsorbents.
PREPARATION OF THE LIGNOCELLULOSIC ADSORBENTSPM, CT, and CM teabags were purchased from a localsupermarket and spent in sequential rinses of boiling distilledwater to extract color, smell, and taste. Final rinses were done withboiling deionized water to remove any residual impurity. Then,the teabags were cut open and the adsorbents were oven-dried ata temperature no higher than 50C to prevent any chemical ofthermal decomposition. Adsorbents were not modified in theirparticle size, as they showed appropriate dimensions for theirdirect use in adsorption experiments. Finally, all adsorbents werestored in plastic containers at room temperature till their usage.No evidence of biological decomposition was observed.
DISCONTINUOUS ADSORPTION EXPERIMENTSBatch experiments were carried out in duplicate at roomtemperature by combining variable masses of the adsorbentswith 50 mL of dye solutions under orbital agitation at 250 rpmfor 24 h. Preliminary studies indicated that less than 24 h areneeded to reach equilibrium. Initial solution pH was adjusteddepending on the type of experiment. Adsorption mixture was
sealed with parafilm to avoid evaporation. Upon equilibrium,the suspensions were separated by gravity and the remainingdye concentration was determined by spectrophotometry, usinga microplate reader (Biotek, Synergy4) at a wavelength of 380 nm.Equilibrium parameters were sequentially optimized, includingpH, mass of adsorbent, initial dye concentration, ionic strength,and presence other pollutants like heavy metals (copper, lead, andzinc divalent ions). After the optimization of each parameter, theywere directly used for the following experiments. Lead, zinc, andcopper salts were utilized in their nitrate forms (Fisher Scientific,reagent grade). Polyethylene glycol (PEG) (MW = 1000 g/mol)was also used as an interfering substance and used without furtherpurification (Spectrum Chemicals, reagent grade). Crowding,salinity, and presence of heavy metal ions were carried using theoptimum pH, the optimum masses and a initial dye concentra-tion of 100 mg/L.
DESORPTION EXPERIMENTSA big-scale adsorption experiment was carried out with all theoptimized equil